ORIGINAL ARTICLE DOI 10.1007/s10086-003-0570-6
Md Iftekhar Shams · Hiroyuki Yano · Keijirou Endou
Compressive deformation of wood impregnated with low molecular weight
phenol formaldehyde (PF) resin I: effects of pressing pressure and pressure
Received: April 25, 2003 / Accepted: August 1, 2003
M.I. Shams (*) · H. Yano
Research Institute for Sustainable Humanosphere, Kyoto University, Gokasho, Uji, Kyoto 611-0011, Japan
Tel. ⫹81-774-38-3670; Fax ⫹81-774-38-3678 e-mail: firstname.lastname@example.org
Wood Research Center of Fukushima Prefecture, Fukushima, Japan Abstract The deformation behavior of low molecular weight phenol formaldehyde (PF) resin-impregnated wood under compression in the radial direction was investigated for obtaining high-strength wood at low pressing pressures. Flat-sawn grain Japanese cedar (Cryptomeria japonica) blocks with a density of 0.34 g/cm3
were treated with aque-ous solution of 20% low molecular weight PF resin resulting in weight gain of 60.8%. Oven-dried specimens were com-pressed using hot plates fixed to a testing machine. The temperature was 150°C and the pressing speed was 5 mm/ min. The impregnation of PF resin caused significant soften-ing of the cell walls resultsoften-ing in collapse at low pressures. The cell wall collapse was strain-dependent and occurred at a strain of 0.05–0.06 mm/mm regardless of whether the wood was treated with PF resin. Thus, pressure holding causing creep deformation of the cell walls was also effec-tive in initiating cell wall collapse at low pressure. Utilizing a combination of low molecular weight PF resin impregna-tion and pressure holding at 2 MPa resulted in a density increase of PF resin-treated wood from 0.45 to 1.1 g/cm3
. At the same time, the Young’s modulus and bending strength increased from 10 GPa to 22 GPa and 80 MPa to 250 MPa, respectively. It can be concluded that effective utilization of the collapse region of the cell wall is a desirable method for obtaining high-strength PF resin-impregnated wood at low pressing pressures.
Key words Low molecular weight PF resin · Pressure hold-ing · Densification · Cell wall collapse
It is desirable in the twenty-first century to build a sustain-able society based on renewsustain-able and sustainsustain-able resources. In this sense, wood may be considered as a future-oriented material even though it is one of the oldest and most common materials. However, dimensional instability due to moisture, low durability caused by biodeterioration, and relatively low mechanical properties of wood and reconsti-tuted wood compared with other engineering materials may prevent wood from replacing materials that are based on unrenewable resources.
To overcome these drawbacks, phenol formaldehyde (PF) resin impregnation and compression seems to be a promising technique. When wood is treated with PF resin and compressed at pressing pressures of 7 MPa or above, its density reaches 1.2 to 1.35 g/cm3
. This product has been given the generic name Compreg and shows high mechanical pro-perties, dimensional stability, and decay resistance.1–4 Because of such properties, much research following on from the work of Stamm’s has been performed, and, in recent years, the potential strength of PF resin-impregnated compressed wood has been extensively studied.5–8 For ex-ample, when wood that was selected based on sound velocity was impregnated with low molecular weight PF resin and hot pressed at a pressing pressure of 50–80 MPa, the bending strength reached 520–530 MPa. Furthermore, when lignin and hemicellulose were removed from the wood and the specimens were impregnated with low molecular weight PF resin and hot pressed at high pressure, the Young’s modulus and bending strength attained 62 GPa and 670 MPa, respec-tively. On the other hand, when PF resin-impregnated wood elements such as particles and powder were hot pressed under high pressure, a decrease in element size did not result in a decrease in bending strength, because high interactive forces developed between elements.9
pressing pressure required during manufacturing becomes a problem. A pressing technique to obtain highly densified wood at lower pressing pressure has to be established. Although many studies on the compressive deformation of wood as a cellular material have been done,10–13
none has clarified the deforming behavior of low molecular weight PF resin-treated wood where PF resin acts as a plasticizer at first and then loses these effects by polymerizing or curing during hot-pressing. Therefore, in this study, compressive deformation of PF resin-impregnated wood was analyzed. Then, a method for deforming wood at lower pressing pressure was studied.
Materials and methods
The raw material was Japanese cedar (Cryptomeria
japonica) with an air-dried density of 0.34 g/cm3
. Flat-sawn grain specimens with dimensions of 60 mm (longitudinal, L) by 40 mm (tangential, T), and 6 mm (radial, R) were cut in a series from the sapwood portion of a block. Average annual rings width was 1.7 mm.
Treatment with phenol formaldehyde resin
Oven-dried specimens were soaked in an aqueous solution of 20% low molecular weight PF resin with an average molecular weight of about 300 (PL 2771, Gun-ei Chemical, pH 5.5, gelation time at 150°C is 10 min). The specimens were kept under vacuum for 12 h, after which release pres-sure and the specimens were kept at room temperature for 12 h. This process was repeated seven times in order to obtain complete penetration of the solution into the wood. After air-drying for 3 days, the treated specimens were vacuum-dried at 50°C for 12 h to remove any residual mois-ture (oven-dried). The weight gain determined using the oven-dried weight before and after treatment was 60.8%.
Measurement of deformation of wood
Two oven-dried specimens were compressed in the radial direction at various pressure levels using hot plates fixed to the Instron Universal Testing Machine (UTM, model 5500) (Fig. 1). This machine allows precise movement of the crosshead thus providing data on how wood can be com-pressed. The crosshead movement, load, and accumulated time were logged using a computer attached to the UTM. After the removal of the deformation of hot plates and their attachments, the deformation of wood in the thickness direction was evaluated.
The pressing speed was 5 mm/min and the pressing temperature was 150°C. After reaching the desired pressing pressure, the crosshead movement was stopped and the condition was kept for 30 min or the pressing pressure held for 30 min (referred as pressure holding). The relationship
between pressing pressure and density was determined based on stress–strain curves.
Evaluation of bending properties
Two specimens with dimensions of 50 mm (L) ⫻ 8 mm (T) were cut from each compressed wood and oven-dried for 6 h at 105°C before measurement of the oven-dried weight and final dimensions. After rounding the cut edges along the length of the specimens with sandpaper (grit #300) to elimi-nate the micro cracks brought about during cutting, the Young’s modulus and bending strength in the oven-dried condition were evaluated by a three-point load bending test with a span of 40 mm using an Instron 4411 universal testing machine at a crosshead speed of 5 mm/min.
Results and discussion
Effects of pressing pressure
pressures, this region is of importance. When most of the cells have been collapsed, the post collapse region begins. The characteristic feature of this region is the densification of wood, with a rapid increase in stress as the compression continues.
As shown in Fig. 2b, PF resin-impregnated wood with a weight gain of 60.8% shows a behavior similar to that of untreated wood. However, PF resin-impregnated wood
requires lower stress to initiate cell wall collapse than untreated wood. For example, to initiate collapse, PF resin-impregnated wood required a pressing pressure of 1 MPa while the untreated wood required a pressure greater than 2 MPa. This indicates that the low molecular weight PF resin in the cell wall acts as a plasticizer and causes signifi-cant softening of the cell wall, inducing a reduction of Young’s modulus of the cell wall in the cross fiber direction. In addition, Fig. 2b shows that a certain strain is required to initiate collapse, irrespective of PF resin-treated or un-treated condition. This result implies that the cell wall col-lapse in the radial direction is strain-dependent rather than stress dependent.
To understand the deforming behavior of wood more clearly, the relationship between pressing pressure and den-sity was evaluated as shown in Fig. 3. Impregnation of PF resin resulted in higher densification, giving a density of 1.35 g/cm3
at a pressing pressure of 10 MPa. However, un-treated wood requires about 30 MPa to attain the same density. Figure 3 also implies that most of the densification occurred in the collapse region. As a consequence, the den-sity of PF resin-impregnated wood increases from 0.47 g/cm3 to 0.92 g/cm3
with increasing pressing pressure from 1 to 2 MPa, which shows that the density increases by around two times by the application of slightly increased pressure. On the other hand, untreated wood could not attain an identical density at a pressing pressure of 2 MPa, because the cell wall collapse does not start until a pressure of above 2 MPa is applied.
In general, the mechanical properties of wood increase with increasing density, due to the increment of volume ratio of the cell wall. Figure 4 shows the Young’s modulus and bending strength of PF resin-treated and untreated wood compressed at different pressing pressures. After reaching the desired pressing pressure level, the crosshead Fig. 2. Typical stress–strain curve of oven-dried wood compressed in
the radial direction at a pressing temperature of 150°C and a pressing speed of 5 mm/min (a) and comparison with phenol formaldehyde (PF) resin-impregnated wood (b)
movement was stopped and the condition was held for 30 min. The Young’s modulus and bending strength increase linearly with increasing density, regardless of PF resin treatment. Furthermore, it was observed that despite the large increment of pressing pressure, that is 2 to 10 MPa (five times more pressing pressure), the increase in density in the post collapse region of PF resin-treated wood was around 1.0 to 1.35 g/cm3
, whilst the improvement in
mechanical properties was small. This means that making use of the collapse region is an effective way, not only for increasing density but also, for increasing mechanical properties of wood.
Effects of pressure holding
Because the occurrence of cell wall collapse was found to be strain dependent, creep deformation of cell walls to initiate collapse at lower pressing pressures was accordingly studied at various pressing pressures ranging from 0.5 to 10 MPa. After reaching the desired pressing pressure, the pressure was held for 30 min as shown in Fig. 5. When PF resin-impregnated wood is compressed at 0.5 MPa, the effect of pressure holding on density can be negligible. However, when wood is compressed at 1 MPa, a significant increment in density occurs during the pressure-holding period. The density increases from 0.52 to 0.84 g/cm3
, which is around 70% higher than the density before pressure holding. At high pressing pressures such as 5 MPa and 10 MPa, the effect of pressure holding on density is not as significant as that at 1 MPa. This result implies that a proper combination of pressing pressure and holding period is needed to obtain marked deformation of wood at lower pressing pressures.
Hence, to understand deformation behavior during pressure holding from the viewpoint of collapse, the stress– strain curve of PF resin-impregnated wood was analyzed as shown in Fig. 6. At a pressing pressure of 0.5 MPa, although wood had already passed the collapse initiating strain of 0.05–0.06 mm/mm, the deformation stopped after a slight increase in strain due to collapse. Contrary to this, a Fig. 4. Effects of low molecular weight PF resin impregnation and
compression on the Young’s modulus and bending strength of wood. Specimens were compressed at different pressing pressures. After reaching the desired pressure, crosshead movement was stopped and the condition was held for 30 min
significant strain increment occurs during pressure holding at 1 MPa. The strain of PF resin-impregnated wood is 0.11 mm/mm at 1 MPa before pressure holding, and in-creases drastically up to 0.45 mm/mm during holding. Com-paring the deforming behavior between pressure holding at 1 MPa and at 2 MPa, it can be seen that the deformation of wood compressed at 1 MPa terminates just before the post collapse region. According to the stress–strain curves of the post collapse region, as shown in Fig. 6, the slope of the curve increases with an increase of strain. It shows that the Fig. 6. Changes in strain during 30 min of holding time under different pressures
Fig. 7. Effect of duration of pressure holding on the densification of PF resin-impregnated wood
resistance of the cell wall against deformation increases with increasing strain at the post collapse region. This suggests that a certain balance between cell wall resistance and applied pressure exists during creep deformation in a collapse-dominant region as well. However, the curing of PF resin may possibly play a role in this case.
To clarify the effects of curing on the deforming behav-ior of PF resin-impregnated wood, changes in density during pressure holding were studied. Figure 7 shows the changes in density within 5 min. It can be seen that within 1 min, the density significantly increases regardless of higher or lower pressing pressures. After a holding time of 1 min, the density was almost consistent. Considering that the gelation time of PF resin used in this study is 10 min at 150°C, the stabilization of density during holding can be attributed to the balance between cell wall resistance and the applied pressing pressure. This suggests that pressure holding of 1 min is enough for the densification of wood at lower pressing pressures as long as the deformed condition is fixed.
The relationships between density and mechanical properties of PF resin-impregnated wood with pressure holding (with creep deformation) and nonholding (without creep deformation) are depicted in Fig. 8. There is no significant difference in mechanical properties between pressure holding and nonholding at the same density. As a consequence, at a pressing pressure of 2 MPa utilizing a combination of pressure holding, the density of Japanese cedar impregnated with low molecular weight PF resin increases from 0.45 to 1.1 g/cm3
. At the same time, the Young’s modulus and bending strength increase from 10 GPa and 80 MPa to 22 GPa and 250 MPa, respectively. It can be concluded that effective utilization of collapse is promising for the production of high-strength wood at low pressing pressures.
The effect of low molecular weight PF resin impregnation on the compressive deformation behavior of wood was in-vestigated. The impregnation of PF resin causes significant softening of the cell walls, inducing a reduction of Young’s modulus and resulting in collapse at lower pressures. The cell wall collapse is strain dependent rather than stress dependent, which results in the densification of wood at lower pressing pressures. Furthermore, the proper com-bination of pressure and its holding results in marked
defor-mation of wood at lower pressing pressures. By addition of pressure holding, even at a pressing pressure of 2 MPa, the density of PF resin-impregnated wood increases from 0.45 to 1.1 g/cm3
and Young’s modulus and bending strength increase from 10 GPa and 80 MPa to 22 GPa and 250 MPa, respectively. Thus, the effective utilization of collapse is a promising technique for the production of high-strength PF resin-impregnated wood at low pressing pressures.
Acknowledgments The authors thank Gun-ei Chemical Industry Ltd for supplying low molecular weight phenol formaldehyde resin. Finan-cial assistance from Ministry of Education, Culture, Sports, Science and Technology, Japan, is greatly appreciated.
1. Stamm AJ, Seborg SM (1955) Forest Products Laboratory resin-treated laminated, compressed wood (Compreg). Forest Product Lab Report 1381 Rev
2. Stamm AJ (1964) Wood and cellulose science. Ronald, New York, pp 343–358
3. Stamm AJ, Bachelor RH (1960) Decay resistance and dimensional stability of five modified woods. Forest Prod J 10:22–26
4. Stamm AJ, Seborg RM (1939) Resin treated plywood. Ind Eng Chem 31:897–902
5. Yano H, Hirose A, Inaba S (1997) High strength wood based materials. J Mater Sci Lett 16:1906–1909
6. Yano H, Ozaki M, Hata T (1997) High strength plastic like com-posites from hardboard. Holzforchung 51:287–288
7. Yano H, Hirose A, Collins PJ, Yazaki Y (2001) Effects of removal of matrix substances as a pretreatment in the production of high strength resin impregnated wood based materials. J Mater Sci Lett 20:1125–1126
8. Yano H (2001) Potential strength for resin impregnated com-pressed wood. J Mater Sci Lett 20:1127–1129
9. Yano H, Mori AK, Collins PJ, Yazaki Y (2000) Effects of element size and orientation in the production of high strength resin impregnated wood based materials. Holzforchung 54: 443–447 10. Bodig J (1965) The effect of anatomy on the initial stress–strain
relationship in transverse compression. Forest Prod J 15:197–202 11. Gibson LJ, Ashby MF (1997) Cellular solids: structure and
proper-ties. Cambridge University Press, Cambridge, pp 278–315 12. Wolcott MP, Kamke FA, Dillard DA (1990) Fundamentals of flake
board manufacture: viscoelastic behavior of the wood component. Wood Fiber Sci 22:345–361